Voltammetry at &,-modified electrodes Voltammetry at &,-modified electrodes Richard G....
Embed Size (px)
Transcript of Voltammetry at &,-modified electrodes Voltammetry at &,-modified electrodes Richard G....
1. Electroanal. Chem., 344 (1993) 235-247 Ekevier Sequoia S.A., Lausanne
Voltammetry at &,-modified electrodes
Richard G. Compton l , R. Anthony Spa&man, D. Jason Riley, R. Geoffrey Wellington, John C. Eklund and Adrian C. Fisher
Physical Chemistry Laboratory, South Parks Road, Oxford, OXI 3QZ (UK)
Malcolm L.H. Green, Richard E. Doothwaite, Adam H.H. Stephens and John Turner
Inorganic Chemistry Laboratory, South Parks Road, Oxford OX1 3QR (UK)
(Received 21 May 1992; in revised form 9 June 1992)
The reduction of electrodes coated with C~fullerene is examined in acetonitrile solution contain- ing a wide variety of supporting electrolytes (MClO,; M = Li, Na, Ba,,s, NR,). Electrochemical intercalation is observed with the formation of fulleride salts. Intercalation is typically irreversible except for the case of R = n-butyl where stable coats of fullerides may be formed into which charge can be passed with near chemical reversibility. Electron-transfer reactions at electrodes modified with C, coatings were investigated for diverse substrates. With unreduced coats impeded diffusion to the metal surface was seen, whereas with films reduced in the presence of tetrabutylammonium perchlorate coat-mediated electron transfer to the substrate was possible.
This paper is concerned with the electrochemical behaviour of thin coats of C, deposited onto an electrode surface and studied voltammetrically using a non- aqueous solvent (acetonitrile) in which C, is essentially insoluble. In a Preliminary note [l] we have reported that the reduction of such coats is strongly dependent on the nature of the supporting electrolyte employed, and that specifically with tetrabutylammonium perchlorate (NBu,ClO,, TBAP) reasonably stable coatings were achievable into which electrons could be (chemically) reversibly injected, presumably leading to the formation of tetrabutylammonium salts of C& anions. Intriguingly, this “electrochemical intercalation” was revealed by two separate voltammetric waves each associated with the uptake of one electron per two C, molecules, suggesting the formation of the salts NBu:(C,), and NBuiC,. In this
l Author to whom correspondence should be addressed.
C!922-0728/93/$06.00 0 1993 - Elsevier Sequoia S.A. Ail rights reserved
paper we (i) report these observations more fully, (ii) extend our voltammetric investigations of f&-modified electrodes to examine a diversity of electrolytes, thus developing the work of Jehoulet et al.  and Chabre et al. , and (iii> examine some electrode reactions taking place at these electrodes. We note that prior work in ref. 2 was unfortunately unreferenced in our Preliminary note [l].
Stable C,, coats with good adhesion characteristics were prepared by evapora- tion of a small quantity of a solution on a gold or platinum electrode. Optimal reproducibility was found to result from the rapid evaporation encouraged by the heating of the electrode achieved using an industrial hot air gun (H.J. Latham Ltd., Shoeburyness, UK). Typically, drops of solution (ca. 3 l.~l) containing C, in dichloromethane (17 or 25 FM), were coated one at a time onto a small insulated metal disc (area, ca. 0.4 cm21 and heated to dryness before the addition of subsequent drops to form a coat of the desired thickness. Other methods of preparation produced modified electrodes with distinctly less reproducible charac- teristics.
Standard voltammetric measurements were made using a Solartron Instruments 1286 electrochemical interface which was combined with a 1250 frequency re- sponse analyser for the purposes of ac impedance studies. Rotating-disc hydrody- namic voltammetry was pursued using Oxford Electrodes equipment. All experi- ments were conducted in outgassed acetonitrile containing 0.1 M supporting electrolyte of the chemical identity specified below. All potentials were recorded against a saturated calomel reference electrode (SCE).
TBAP, tetraethylammonium perchlorate (TEAP), tetrahexylammonium per- chlorate (TI-IAP), tetraoctylammonium perchlorate (TOAP), lithium perchlorate and barium perchlorate were obtained from Fluka. Sodium perchlorate and N,N,N’,.N’-tetramethylphenylene diamine (TMPD) were supplied by Aldrich. Lancaster Synthesis provided tetrabromo-p-benzoquinone (“p-bromanil”, PBA) and methylene blue (MB) was purchased from Sigma. 9,10-Anthraquinone (AQH) and N-phenyl-p-phenylene diamine (PPPD) were obtained from BDH Ltd.
RESULTS AND DISCUSSION
First we consider the cyclic voltammetric responses seen from gold electrodes modified by “thin layers” of C, formed by the evaporation of no more than a total of 100 ~1 of 25 PM solution of fullerene under conditions fulfilling the experimental protocol described in the previous section. This leads to surface coverages of 6.5 X 10e9 mol cmp2 corresponding to coats of thickness of ca. 40 monolayers or less. The electrodes were examined in acetonitrile solution contain- ing a wide variety of different supporting electrolytes present at a concentration of 0.1 M. The results are shown in Figs. 1, 2 and 6 which all relate to a voltage scan rate of 100 mV s- ’ and can be summarized as follows.
Fig. 1. Cyclic voltammograms showing the electroreduction of a “thin-layer” &-modified electrode in 0.1 M supporting electrolyte: (a) LiCIO,; (b) Ba(CIOJ,; (c) NaClO,. In all three cases a scan rate of 100 mV s-* was used.
Lithium, sodium and barium per-chlorates
Figure 1 shows the first and second scans resulting from potential cycling within the windows encompassing all the fullerene-related faradaic features in each case. Large reduction waves are seen on the first negative scan, and integration of these curves shows that for all three systems a total of one electron (with a maximum error of + 10%) per Cm ball is passed; the shape of the voltammograms is suggestive of electron transfer to a surface-immobilized layer [41. Only very small oxidative currents pass on the reverse (positive) voltage sweep and all faradaic activity is completely lost after a second potential cycle. We infer the (chemically) irreversible electrochemical intercalation of C, with the formation of the salts M+C; (M = Li, Na) and Ba2+(C&. We return to these observations below.
Fig. 2. Cyclic voltammograms showing the electroreduction of a “thin-layer” C&-modified electrode in 0.1 M supporting electrolyte: (a) TEAP; (b) THAP; (c) TOAD’. Scan rate, 100 mV s-‘.
Tetra-alkylammonium perchlorates NR:CIo,- (R = ethyl, n-he&, n-octyl)
Figure 2 shows the first potential cycle obtained in each case for potential limits embracing all Cm-related features; in subsequent cycles only negligible faradaic currentsare visible. Significant oxidative processes are absent on the first reverse scan provided that the first reductive scan includes the final fullerene-related peak in each case, as in the voltammograms shown in Fig. 2. If the cyclic voltammogram is reversed before the final peak, one or more small oxidative features may be observed, but in all cases cycling the voltammogram a second time reveals no substantial reproducible faradaic electrochemistry (either reductive or oxidative). Integration of the total charge which may be injected into the coat (sum of all reductive voltammetric peaks) suggests that between two and three electrons per C, are transferred. We note that superconducting salts of the stoichiometry M,C, (M = K, Rb, Cs) have been made by chemical synthetic routes [5,61.
For TEAR, integration of the three peaks seen (see Fig. 2(a)) shows that close to two electrons per C, in total are passed into the coat. Figure 3 shows that this number is insensitive to the coat coverages in the range 1 x 10d9-6 X 10m9 mol cmm2 and provides a good indication of the level of certainty which can be obtained in the measurements described and hence in the reproducibility of the method of preparing the C, coatings. Also shown in Fig. 3 is an indication of the
C0v2erage3xl 0Glol cm5-2
Fig. 3. The number of electrons injected into the C, coat when reduced in acetonitrile + 0.1 M TEAP
measured as a function of fullerene coverage in all voltammetric peaks CO), in peak A (A ), in peak B
(+) and in peak C(X).
charge passed in each of the peaks, although the level of voltammetric complexity revealed in Fig. 2(a) shows that these estimates are necessarily very approximate.
For THAP, integration of all four peaks gives a total electron injection close to three electrons per fullerene as shown in Fig. 4. Also shown are the charge injections for peaks A, B + C and D. In the case of TOAP just two peaks are discernable. Figure 5 shows the charge injected per peak and the total charge injection as a function of surface coverage. AC impedance measurements made before reduction of the coat in the presence of THAP revealed essentially
3.0 - n 0
E - ” d
” 2 0
$ 2.0 - 5 *
+ T . +
z _ +
n E i.o- z’ I A ,,
ti 0 y A A A L
x = * A * A x I I I 1 L I 1 6
Fig. 4. The number of electrons injected into the Cm coat when reduced in acetonitrile + 0.1 M THAP
measured as a function of fullerene coverage in all voltammetric peaks CO), in peak A (A), in peaks
B + C c